Effects of SO2 Shielding Gas Additions on GTA Weld Shape
Small additions of SO2 in argon shielding gas for GTA welding both suppresses variability and improves joint penetration in 21-6-9 and 304 stainless steels
BY C R. HEIPLE AND P. BURGARDT
ABSTRACT. Substantial increases in GTA joint penetration, can vary substantially For pure metals and many alloys, the weld depth/width ratio resulted from between different heats (and even within surface tension decreases as temperature small additions of sulfur dioxide (S02) to the same heat) of material with the same increases (Ref. 2). For weld pools in such the torch shielding gas when welding two nominal composition. materials, the surface tension will be stainless steels. The improvement was Heiple and Roper (Ref. 1) have recently greatest on the coolest part of the pool demonstrated on both Types 304 and proposed a mechanism for the origin of surface at the edge, and lowest on the 21-6-9 austenitic stainless steels, but variable GTAW joint penetration by hottest part under the arc near the center would be expected for iron-base alloys which weld pool shape can be substan of the pool. Such a surface tension gradi generally. The weld pool shape achieved tially altered by variations in the concen ent produces outward surface fluid flow was essentially independent of variations tration of certain trace elements in the (as shown schematically in Fig. 1A) and in both SO2 content of the torch gas and weld pool. They proposed that the major generates a relatively wide and shallow base metal composition when SO2 in the factor determining weld shape is general weld. shielding gas was in the range of 500 to ly fluid flow in the weld pool and that, Surface-active trace elements, when 1400 ppm. With 700 ppm S02 in the under many common GTA welding con present in sufficient quantity in the weld torch gas, less than 30 ppm sulfur was ditions, the major factor driving fluid flow pool, create a positive surface tension added to an autogenous weld bead. For is a surface tension gradient. Trace ele temperature dependence (Ref. 2). Under alloys where this additional sulfur can be ments affect weld pool shape by altering these conditions, the surface tension will tolerated and appropriate measures can surface tension gradients, thereby chang be highest near the center of the weld be taken to handle the toxic SO2, this ing the magnitude and/or direction of pool and an inward surface fluid flow technique offers a promising way to fluid flow in the weld pool. results (as shown schematically in Fig. 1B). improve GTA weld joint penetration while suppressing variable penetration.
Introduction The shape of GTA welds has long been of concern, in part because the GTA welding process tends to be used in applications where high quality, high pre cision welds are required. Furthermore, the welds are often made by automatic equipment, which is presently unable to compensate for variability in weld pool geometry once the welding variables have been set. For these reasons, consid WELDING erable interest has been generated by the DIRECTION observations that weld shape, especially
Paper presented at the AWS 66th Annual Convention, held April 28-May 3, 1985, in Las Vegas, Nev.
C. R. HEIPLE is in Physical Metallurgy R&D and P. BURGARDT is in Nuclear joining R&D at B Rockwell International, Rocky Flats Plant, North Fig. 1 — Proposed (Ref. 1) surface ana subsurface fluid flow in the weld pool. A —surface tension American Space Operations, Golden, Colo. temperature coefficient negative; B — surface tension temperature coefficient positive
WELDING RESEARCH SUPPLEMENT 1159-s This fluid flow pattern produces relatively The second experiment was designed welding conditions for both the experi deep, narrow weld beads. to determine if variable joint penetration ment with varying S02 shielding gas con In iron-base alloys, sulfur and oxygen could be suppressed with S02 shielding tent and the experiment with doped base are the surface-active trace elements gas additions. Strips in a 17 mm (0.67 in.) metal were: current— 150 A DCEN; elec most commonly present. Historically, sul thick plate of 304L stainless steel were trode to work distance —2 mm (0.080 fur and oxygen levels have been high doped with either sulfur or selenium, and in.); travel speed— 150 mm/min (6 ipm); enough so that complete joint penetra GTA welds were subsequently passed electrode tip angle —45 degrees; and tion was observed consistently, i.e., weld across the doped zones and undisturbed shielding gas flow rate —0.57 m3/hr (20 depth/width (d/w) ratios of about 0.5. base metal. The doping technique cfh). Finally, both autogenous welds and However, improvements in steelmaking involved electron beam melting foils of welds with cold filler metal addition were practice have made available steels, par 303 stainless steel (for sulfur doping) and made on several joint configurations to ticularly stainless steels, which have 303 Se stainless steel (for selenium dop confirm that the changes observed in extremely low sulfur and oxygen con ing) into the base plate. The addition of bead-on-plate welds would also be seen tents (less than 10 ppm each). Such steels sulfur (Ref. 3) and selenium (Ref. 4) to in full joint penetration welds. exhibit poor joint penetration in GTA stainless steel is known to drastically welding and can have weld d/w ratios as increase GTA weld d/w ratio when the Results low as 0.15. These wide, shallow weld steel has an initially low d/w ratio. The pools create a number of significant doping procedure has been described in SO2 in the shielding gas had a substan welding problems. detail previously (Ref. 5). The 304L plate tial effect on weld pool shape. Weld d/w used in this experiment had an exception One approach to improving GTAW ratio is plotted versus torch gas SO2 ally low sulfur and oxygen content and joint penetration and reducing variable content in Fig. 2. Cross sections of welds exhibited a d/w ratio of about 0.17. The joint penetration is to add small concen made using pure argon and 750 ppm S02 composition is given in Table 2. It was trations of surface active elements to the are shown in Fig. 3. One of the encour chosen to give the largest possible differ weld pool. This can be accomplished in a aging aspects of the results presented in ence in weld shape between the doped number of ways, including the addition of Fig. 2 is that there is a substantial range zones and undoped base metal. The a doped filler metal wire to the weld (approximately 500-1400 ppm) of S02 pool, coating the joint prior to welding, contents for which the d/w ratio is inde and doping the shielding gas delivered pendent of SO2 concentration. This can through the torch. The additions need to be small, since most elements known to Table 2—Analysis of 304L Plate, wt-% be surface active in iron (S, Se, and Te) promote hot cracking. We report here Cr 19.0 the effects of small SO2 shielding gas Ni 10.3 Table 3 —Sulfur Contents of Welds on additions on GTA welds on 21-6-9 and Mn 1.9 21-6-9, ppm 304 austenitic stainless steels. C 0.034 Al 0.002 Argon Argon + Argon + o 0.001 2 Shield 750 ppm 2000 ppm S02 Experimental S 0.002 so2 Fe balance 40 67 150 The initial experiment consisted of pro ducing GTA bead-on-plate welds on a 25 mm (1 in.) thick plate of 21-6-9 stainless steel. Since the intent of the experiment was to determine if S02 additions to the torch gas would improve weld d/w ratio, a plate with known-poor d/w ratio was used. The composition of the plate is given in Table 1. All welds were made under identical welding conditions except that the torch gas composition was va ried between pure argon and argon con taining 2000 ppm S02. The welding was performed in a large chamber filled with argon. The SO2 content in the shielding gas was varied by mixing pure argon with gas from a second cylinder containing argon with 2000 ppm SO2.
Table I—Analysis of 21-6-9 Plate, wt-%
UJ Cr 20.1 >UJ Ni 6.8 Q Mn 8.7 X N2 0.27 O C 0.025 200 400 600 800 1000 1200 1400 1600 1800 2000 tr Al 0.0058 TORCH GAS S02 < 02 0.0058 CONTENT, ppm cUoJ S 0.0024 UJ Fe balance Fig. 2 - Effect of sulfur dioxide in the shielding gas on GTA weld depth/width ratio. 21-6-9 stainless steel
160-slJUNE 1985 0.5
S ft X ' o \ 0.4 - / O \ i l I \ I \ t i a 0.3 D -i A UJ £ \ \ N 0.2 o
0.1 a 100 AMPS O 150 AMPS Fig. 3-Cross sections of GTA welds made A 200 AMPS with (top) pure argon shielding gas and (bot tom) argon plus 750 ppm 502 shielding gas I J_ 500 1000 1500 2000 TORCH GAS OXYGEN be contrasted with the results obtained in CONTENT(PPM) a similar experiment when oxygen was Fig. 4-Effect of oxygen in shielding gas on GTA weld depth/width ratio (Ref. 6) added to the shielding gas, where a relatively sharp maximum in d/w ratio is obtained with increasing oxygen concen tration—Fig. 4. Welds made with shield was added to the weld; the increase was gas additions, are shown in Fig. 5. Base ing gas of pure argon, 750 ppm S02, and only 25 ppm with 2000 ppm S02 in the metal containing welds with d/w ratios, 2000 ppm S02 were cut from the plate shielding gas. which differed by a factor of more than and analyzed for sulfur and oxygen. The The results of the second experiment, two with argon shielding, exhibited near measured sulfur contents of the welds to determine if variable joint penetration ly identical weld shape when welded are given in Table 3. Very little oxygen would be suppressed by SO2 shielding with 700 ppm SO2 in the shielding gas. Thus, the same weld pool shape can be achieved independent of base metal chemistry variations. The dramatic increase in bead-on-plate weld d/w ratio observed when S02 was added to the shielding gas was also observed for welded joints. Figure 6 is a cross section of a welded butt joint in O which a portion of the weld (Fig. 6A) was produced using argon shielding gas and < the other portion (Fig. 6B) was made using 700 ppm SO2 in the shielding gas. **a* Similar results are obtained in welds with T3 cold filler metal addition —Fig. 7. In both Q _J cases, the other welding variables were UJ the same for both sections of the weld.
Discussion Previous work has demonstrated that sulfur and other surface-active element additions increase the d/w ratio of GTA welds on ferrous alloys (Ref. 3). The increase is predicted by the surface ten sion-driven fluid flow model (Ref. 1) and arises from changes caused by the sur TORCH GAS S02 face-active elements in surface tension CONTENT, ppm gradients. Sulfur is generally undesirable Fig. 5 — Effect of shielding gas SO2 content on the changes in GTA weld depth/width ratio causedin steels, causing or contributing to by 304L base metal chemistry variations (among other things) increased inclusion
WELDING RESEARCH SUPPLEMENT 1161-s Furthermore, if heats of stainless steel with joint penetration characteristics that differ when welded in argon are welded with S02 in the torch gas, the joint penetration is improved and the weld shape is essentially indistinguishable for the different heats. Similar results are anticipated for other stainless steels and ferrous alloys, generally. The maximum benefit from SO2 additions is achieved between about 500 and 1400 ppm. Fig. 6 - Welded butt joints on 304L stain/ess steel with (left) pure argon and (right) argon plus 700 Under a common GTA welding condition ppm SO2 shielding gases. All other welding variables were unchanged; the SO2 was simply turned(15 0 A, 150 mm/min/6 ipm travel speed), off when the weld was partially completed. Current — 47 A; travel speed — 200 mm/min less than 30 ppm sulfur is added to the 21-6-9 stainless steel when there is 700 ppm S02 in the shielding gas. When appropriate measures to handle the toxic SO2 can be taken, this technique offers a promising way to improve joint penetra tion in GTA welding and to suppress variable joint penetration. The only torch gas dopants which we have tested are oxygen and SO2; however, it is possible that other dopants could be found which would be as successful or, more so.
A ckno wledgment This work was supported by the Department of Energy, Albuquerque Fig. 7— Welded butt joints on 304L stainless steel using 308 filler metal wire with (left) pure argonOperation s Office. Its support is grateful and (right) argon plus 700 ppm SO2 shielding gases. All other we/ding variables were unchanged;ly acknowledged. the SO2 was simply turned off when the weld was partially completed. Current— 163 A; travel speed— 130 mm/min; feed speed of 0.045 in. wire —750 mm/min References 1. Heiple, C. R., and Roper, |. R. 1982. content, hot cracking and reduced safely remove the gas are therefore Mechanism for minor element effect on GTA toughness. There has therefore been a required. It is also an environmental haz fusion zone geometry. Welding journal61(4): 97-s to 102-s. major effort, with considerable success, ard and, if used in significant quantities, 2. Allen, B. C. 1972. The surface tension of to lower sulfur levels in steels. Unfortu would require treatment. The weld bead liquid metals. Liquid Metals-Chemistry and nately, this can lead to significant GTA surface is discolored when welding is Physics, ed. S. Z. Beer: 161-212. New York: M. welding problems. The addition of small performed with S02 in the shielding gas, Dekker, Inc. concentrations of sulfur to the weld pool which may be unacceptable for certain 3. Heiple, C. R., and Roper, |. R. 1982. offers one approach to solving the weld applications, although the surface is easily Effects of minor elements on GTAW fusion ing problem without raising the general cleaned. In the limited number of experi zone shape. Trends in Welding Research in the sulfur level in the steel. Mixing about 700 mental welds so far attempted, there has United States, ed. S. A. David: 489-520. Metals Park, Ohio: Am. Soc. for Metals. ppm S02 in shielding gas for GTA weld been no unusual deterioration of the ing improves joint penetration substan tungsten electrode noted; however, it is 4. Heiple, C. R., and Roper, J. R. 1981. Effect tially in austenitic stainless steel, eliminates possible that electrode life would be of selenium on GTAW fusion zone geometry. Welding journal 60(8): 143-s to 145-s. the sensitivity to minor variations in base reduced in a production welding opera 5. Heiple, C. R., Roper, J. R., Stagner, R. T., metal trace element content, and adds tion. Finally, argon-S02 mixtures are not and Aden, R. J. 1983. Surface active element less than 30 ppm sulfur to the weid. at present routinely available, although effects on the shape of GTA, laser, and elec Where this additional sulfur can be toler they can be obtained commercially. tron beam welds. Welding journal 62(3): 72-s ated, this technique appears to be a to 77-s. promising approach to eliminating poor 6. Heiple, C. R„ Burgardt, P., and Roper, ). and variable joint penetration in GTA Conclusions R. 1984. The effect of trace elements on GTA welding. weld penetration. Modeling of Casting and The addition of small concentrations of Welding Processes II, eds. J. A. Dantzig and J. There are potentially significant prob S02 to the normal argon shielding gas T. Berry: 193-205. Warrendale, Pa.: TMS- lems in using S02 in the weld shielding drastically improves the GTA weld d/w AIME. gas. Sulfur dioxide is toxic, with permissi ratio (increases joint penetration) on 304L 7. Sax, N. I. 1984. Dangerous Properties of ble concentrations (Ref. 7) far below the and 21-6-9 stainless steels with initially Industrial Materials, 6th Edition: 2486-2487. levels required for welding. Provisions to poor joint penetration characteristics. New York: Van Nostrand Reinhold Co.
162-s I JUNE 1985